supercapacitor electrodes with integrated high energy ... elimination of heteroatom groups from...
Post on 26-Jul-2020
Embed Size (px)
Renewable Graphene-Like Nitrogen-Doped Carbon Nanosheets as Supercapacitor Electrodes with Integrated High Energy–Power Property
Weiqian Tian, a Qiuming Gao,a* Liming Zhang,b Chunxiao Yang,a Zeyu Li,a Yanli Tan,a Weiwei Qiana and Hang Zhanga
a Key Laboratory of Bio-inspired Smart Interfacial Science and Technology of Ministry of Education, Beijing Key Laboratory of Bio-inspired Energy Materials and Devices, School of Chemistry and Environment, Beihang University, Beijing100191, P. R. China.
b Key Laboratory of Wooden Material Science and Application of Ministry of Education, Beijing Key Laboratory of Lignocellulosic Chemistry, School of Material Science and Technology, Beijing Forestry University, Beijing 100083, P. R. China.
*Corresponding author: Qiuming Gao, E-mail: firstname.lastname@example.org.
Figure S1. The FESEM images of shrimp shell (a) and RGNC (b).
Electronic Supplementary Material (ESI) for Journal of Materials Chemistry A. This journal is © The Royal Society of Chemistry 2016
Figure S2. TGA and DTG curves of dried shrimp shells. The first weight loss around 200oC is ascribed to the exclusion of
adsorbed water. The second (300-400oC) and third (around 700oC) weight losses are mainly the decomposition of
biopolymers to chars. With the temperature higher than about 750oC, the gradual weight loss is attributed to the
elimination of heteroatom groups from chars. The carbonization temperature is the key factor for pore structures and
nitrogen-doped content of result carbons. The carbons with a good balance of surface area and nitrogen content may be
obtained at 800oC.
Figure S3. FETEM images at the edge of chars from carbonized shrimp shell. The chars were obviously embedded by hard
phases of laminated or granular calcium carbonates as the template and auto-activation agents, which can be successfully
removed by washing with dilute acid.
Figure S4. XPS analyses of the chars carbonized from shrimp shell, RGNC and RGNC-NS. The chars carbonized from shrimp
shell contain mainly carbons (285 eV), nitrogen (400 eV) and oxygen (532 eV), as well as calcium (348 eV) and phosphorus
(133 eV) from the calcium carbonate and slight hydroxyapatite. Those inorganic salts were removed by washing with dilute
acid, confirmed by the XPS curves of RGNC and RGNC-NS without the calcium and phosphorus peaks.
Figure S5. The C 1s and N 1s spectra of RGNC. As shown in the deconvoluted C1s spectrum, the high percentage of sp2 C
indicates that the conjugated graphitic domains are built successfully during the carbonization process. The C-N peak
demonstrates the successful incorporation of nitrogen groups to carbon framework. The percentage of different nitrogen
groups is shown in Table 2.
Figure S6. CV curves and charge-discharge voltage profiles of the RGNC-NS-SC (a and c) and RGNC-SC (b and d) in 6 M KOH.
To avoid the overestimation of the specific capacitance for the samples, only the upper half of the discharge curves was
used to determine the capacitance value. As a result, in aqueous electrolyte the RGNC-SC exhibits a specific capacitance of
219 F g-1 at a low current density of 0.5 A g-1 lower than a value of > 330 F g-1 that was calculated from the whole discharge
curve. The outcome is attributed that the lower half of the discharge voltage profile is obviously distorted (Figure S6d)
because of the existence of pseudocapacitance in consistent with the CV analysis (Figure S6b). Whereas, a high specific
capacitance of 322 F g-1 at 0.5 A g-1 was obtained for RGNC-NS-SC due to the more linear discharge voltage profile (Figure
The nearly rectangular CV curves and symmetrically linear charge/discharge voltage profiles of RGNC-NS-SC even at high
rates (Figure S6a and c) indicate a mainly significant capacitance contribution from the double-layer capacitance
superimposed with a partial pseudocapacitance.[S1-S3] The observation is further confirmed by the EIS analysis of RGNC-NS-
SC with a most vertical curve in low-frequency region indicating a significant double-layer capacitance behavior (Figure
3e).[S1] The less than 5% capacitance loss and close 100% Coulombic efficiency after 20 000 cycles at 10 A g-1 was obtained
for RGNC-NS-SC, also demonstrating that the outstanding performance is not mainly ascribed to parasitic reactions.[S4] This
is attributed that the high-aspects-ratio graphene-like structures with a good integration of specific surface area (1946 m2 g-
1) and nitrogen-doped content (8.75 wt.%) in the RGNC-NS can enhance ionic/electronic transports and surface charge
storage capacity, a feature which is still desired in synthesis of advanced nitrogen-doped supercapacitor electrodes.[S2] The
results are consistent with the observation of reported nitrogen-doped carbon nanocages (7.9% N and 1794 m2 g-1 specific
surface area)[S1] and nitrogen-doped mesoporous few-layer carbons (8.2~11.9% N and ~1580 m2 g-1 specific surface area),[S3]
which also show rectangular CV curves and symmetrically linear charge-discharge voltage profiles in symmetric two-
electrode basic electrolyte systems.
In contrast, RGNC-SC exhibits the quasi-rectangular CV curves with one pair of prominently wide redox peaks (Figure S6b)
and curved charge/discharge voltage profiles under 0.5 V (Figure S6d) at low rates but severe distortion at high rates,
indicating a major capacitance contribution from pseudocapacitive which is inefficient in the symmetric electrochemical
system.[S3, S5] The outcome is further confirmed by EIS analysis with a distorted curve in low-frequency region and large EDR
(Figure 3e). It is attributed to the RGNC with high nitrogen-doped content (9.04 wt.%) but low specific surface area (446 m2
g-1). Furthermore, a high content of pyridinic nitrogen of 36.04% was achieved for RGNC compared with 25.55% for RGNC-
NS based on the deconvolution of XPS N1s spectrum (Table 2). The pyridinic nitrogen could generate more
pseudocapacitance effects than the other nitrogen functionalities due to only two electrons involved in the electrochemical
process.[S5, S6] The higher heteroatom-doped content of 16.2 wt.% was also obtained for RGNC than 15.3 wt.% for RGNC-NS
(Table 2). These observations are in agreement with reported carbonized eggshell membrane (8% N and 221 m2 g-1
specific surface area)[S7] and nitrogen-doped porous carbon monolith (11.9% N and 679 m2 g-1 specific surface area).[S6]
Figure S7. (a) The area-normalized capacitances, and (b) electrode specific capacitance Celectr versus square root of
charge/dischage time of the RGNC-NS-SC and RGNC-SC in 6 M KOH at current densities from 1 to 100 A g-1.
The area-normalized capacitances Carea were calculated using the formula Carea = Celectr/SBET, where Celectr is the electrode
specific capacitance and SBET is the specific surface area of active electrode materials. The area-normalized capacitance of
RGNC-NS-SC is to 12.4-16.5 µF cm-2 (Figure S7a), which is well comparable to the theoretical double-layer capacitance of 15-
25 µF cm-2.[S7, S8] But the area-normalized capacitance of RGNC-SC is obviously higher than 49.5-16.3 µF cm-2 (Figure S7a)
due to a low SBET value and a primary capcitance contribution from pseudocapacitance, which is in good agreement with
same reported nitrogen-doped carbons, e.g., egg white-derived carbon of 48.5-29.1 µF cm-2,[S8] and melamine-
derived carbon of 441-33 µF cm-2.[S9]
The charging/discharging kinetic analysis was shown in Figure S7b. The electrode specific capacitance Celectr can take the
form of Celectr = k1 + k2t1/2 where k1 is a rate-independent component for reversible supercapacitance and k2t1/2 is a diffusion-
limited component controlled by the charge/dischage time t (s).[S3] The k1 can be obtained at the t1/2 = 0 intercept with the
vertical axis. As showing in Figure S7b, the rate-independent component k1 of RGNC-NS (~275 F g-1) dominated the total
Celectr, giving a high rate capability. However, the rate-independent component k1 (< 140 F g-1) of RGNC is obviously lower
percentage in total Celectr, further suggesting the dominance of diffusion-limited component. Thus an obviously high rate
capability of 75% was obtained for RGNC-NS-SC (holding 241 F g-1) compared with 33% for RGNC-SC (holding 72 F g-1) at a
high current density of 100 A g-1.
Figure S8. The charge/discharge voltage profiles of RGNC-NS-SC at a low current density of 0.5 A g-1 in the IL
mixture electrolyte under different operating voltage windows from 2.5 to 4 V. The corresponding Coulombic efficiencies
are of 99.8% for 2.5 V, 98.5% for 3 V, 81.3% for 3.5 V and 59.6% for 4 V, respectively.
Figure S9. (a) The charge/discharge voltage profiles at 0.5 A g-1, (b) charge/discharge voltage profiles at current
densities from 0.5 to 20 A g-1, (c) CV curves at scan rates from 100 to 2000 mV s-1, and (d) weight-normalized specific
capacitances for RGNC-SC in the IL mixture electrolyte.
Using the operating voltage window of 3 V, a highl